# Temperature dependence of the electrical transport properties in few-layer graphene interconnects

- Yanping Liu
^{1}, - Zongwen Liu
^{2}, - Wen Siang Lew
^{3}Email author and - Qi Jie Wang
^{1, 4}Email author

**8**:335

https://doi.org/10.1186/1556-276X-8-335

© Liu et al.; licensee Springer. 2013

**Received: **29 May 2013

**Accepted: **11 July 2013

**Published: **25 July 2013

## Abstract

We report a systematic investigation of the temperature dependence of electrical resistance behaviours in tri- and four-layer graphene interconnects. Nonlinear current–voltage characteristics were observed at different temperatures, which are attributed to the heating effect. With the resistance curve derivative analysis method, our experimental results suggest that Coulomb interactions play an essential role in our devices. The room temperature measurements further indicate that the graphene layers exhibit the characteristics of semiconductors mainly due to the Coulomb scattering effects. By combining the Coulomb and short-range scattering theory, we derive an analytical model to explain the temperature dependence of the resistance, which agrees well with the experimental results.

### Keywords

Graphene Graphene multilayer Short-range scattering theory Coulomb scattering effect## Background

Graphene has been a subject of intense research since it was discovered in 2004 because of its intriguing band Structure [1, 2]. The energy-momentum relationship of graphene is found to be linear for low energies near the six corners of the two-dimensional (2D) hexagonal Brillouin zone [1–4], leading to a zero effective mass for electrons and holes [2–5]. Such behaviour can be described by the Dirac equation for spin 1/2 particles [1–6]. Furthermore, graphene is also an excellent electronic material as it can be either a metal or semiconductor depending on the edge states, zigzag or armchair [7]. It exhibits superior mobility, with reported values in excess of 15,000 cm^{2} V^{−1} s^{−1}[1], which is superior to that of III-V semiconductors for high-speed device applications. As such, graphene has been widely predicted to be a potential material for post-complimentary metal-oxide semiconductor technology, particularly for use as ballistic transistors or interconnects [8–12]. Most graphene studies have focused on monolayer structures [1]. Recently, few-layer graphene (FLG) have received much attention because of its promising bandgap tunability. For instance, bilayer graphene is reported to have a tunable bandgap [13, 14] and trilayer graphene is a semimetal in the ideal case with a gate-tunable overlapped bandgap [15]. As more graphene layers are added, the electrical properties of FLG also change, which can be further explored for the design of various devices [15]. However, theoretical understanding and experimental investigations of FLG are still lacking for applications such as interconnect.

In this letter, we report a systematic investigation of the temperature dependence behaviour of the four-terminal electrical resistance in FLG interconnects. The resistance of tri- and four-layer graphene, under direct current (DC) electric fields and in a temperature range from 5 to 340 K was measured. The T^{-1/2} dependence shows the evidence of the electron–electron Coulomb interaction in FLG. Our temperature-dependent resistance results reveal that the FLG interconnects display semiconductor properties and further confirm that Coulomb interaction can play a dominant role.

## Methods

_{2}substrate. The number of graphene layers was confirmed by micro-Raman spectroscopy through the 2D-band deconvolution procedure [16]. The Raman spectra of the graphene structures were measured at room temperature using a WITec CRM200 instrument (Ulm, Germany) under a 532-nm excitation wavelength in the backscattering configuration [16, 17]. Shown in Figure 1 is the Raman spectrum with clearly distinguishable G band and 2D band. The number of graphene layers is distinguished from the full-width half maximum of the 2D band peak [17]. Optical photolithography technique was used to pattern four terminal Cr/Au contact pads on the graphene structures. The metallic contact electrodes of Cr and Au films of thickness 5 and 80 nm, respectively, were deposited using thermal evaporation techniques at a vacuum pressure of 2 × 10

^{−7}mbar. Electronic transport measurements were performed on multiple samples, using the physical property measurement system (PPMS, Quantum Design, San Diego, CA, USA) with a fixed excitation current of 0.01 mA; the temperature varied from 5 to 340 K.

## Results and discussion

*I-V)*characteristics at different temperatures of (a) tri- and (b) four-layer graphene interconnects. Insets show the enlargement of the measurement results at low electric fields. For the tri- and four-layer graphene, the interconnect resistors display two distinct regions of ohmic characteristic: one at fields larger than 0.01 V/μm but less than 0.10 V/μm and the other at fields larger than 0.10 V/μm. The nonlinear behaviour of current–voltage characteristics at low threshold (<0.10 V/μm), and the second ohmic region in the strong DC electric field (>0.10 V/μm) can be explained by the heating effect [18]. Within a strong DC electric field, the relaxation grows sharply with heating, and the recombination of carriers is dominant as compared to thermal generation [18, 19]. At sufficiently high DC electric field, we observe linear

*I-V*over the whole temperature measurement range.

*G*

_{ d }=

*dI*/

*dV*of (a) tri- and (b) four-layer graphene as function of the temperature

*T*

^{−1/2}on a semi-logarithmic scale. As shown in the Figure 3, we can see the experiment results can be well fitted with the Efros-Shklovskii (ES) variable-range-hopping (VRH) model at the low DC electric field. One should note that, for the high electric field conductance, the fitted line shows some deviation from the model due to the heating effect. Therefore, our data suggest that Coulomb scattering is the main scattering mechanism in our device.

*E*. Shown in Figure 4 are the dimensionless resistance

*R*

_{ T }/

*R*

_{T = 5K}as a function of the electric field

*E*at different temperatures, for (a) tri- and (b) four-layer graphene interconnects. Insets display the optical micrographs of the FLG interconnect. At a lower temperature range of 5 to 50 K, as the electric field increases from 0 to 0.6 V/μm, the resistance of the tri- and four-layer graphene interconnects show a reduction of about 30% and 70%, respectively. However, for the temperature range

*T*≥ 200 K, the corresponding resistance drop is smaller. The larger drops of the resistance at lower temperature range indicate that Coulomb scattering is the main transport mechanism in the FLG interconnects at this temperature range as it is proportional to the carrier density. Hence, Coulomb scattering is strongly dependent on temperature. We further note that with increasing temperature, the observed results indicate that the scattering induced by electric field from the substrate surface polar phonons is significantly screened by the additional graphene layers at room temperature [21, 22].

*R*

_{ T }/

*R*

_{T = 5K}, whereby we investigate the temperature dependence change of the resistance. In Figure 5, we present the electrical resistance of the three and four layers of graphene interconnects as a function of temperature. The results show that an appreciable monotonic increase of

*R*

_{ T }/

*R*

_{T = 5K}is observed for decreasing temperature for both the tri- and four-layer graphene. This

*R-T*behaviour indicates that the carriers transport in the graphene layers is non-metallic in nature. This implies that, the resistance does not originate from thermal activation but is attributed to ES VRH between localized states induced by the charge impurities [20–23]. This is the further evidence that the electron–electron Coulomb interaction effects are prominent in such system. As the temperature is reduced from 340 to 5 K, the increase of the four-layer graphene resistance is much larger, which is around 40%, compared to the trilayer graphene, which is found to be 20%.

_{2}-graphene interface, and the short-range scattering is constant. Then the energy average scattering time is deduced as [21, 22]:

where *E*_{
k
} is the wave vector energy and *τ*(*E*_{
k
}) is the transport scattering rate. For the low temperature limit, the scattering time averaged over energy can be written as 〈*τ*〉 ≈ *τ*(*E*_{
F
}) [21]. The density of states *D*(*E*_{
F
}) in tri- and four-layer graphene is assumed to be a constant $D\left({E}_{F}\right)=\frac{2{m}^{*}}{\pi {\hslash}^{2}}$. Here, the Fermi energy is ${E}_{F}=\frac{{\hslash}^{2}{k}^{2}}{2{m}^{*}}=\frac{{\hslash}^{2}\mathit{\pi n}}{2{m}^{*}}$, and based on the Boltzmann equation of mobility as function of the scattering time: $\mu =\frac{\mathit{eD}\left({E}_{F}\right){v}_{F}^{2}\left(\tau \right)}{2n}$, we can obtain the mobility of graphene as ${\mu}_{3-4\mathit{layers}}=\frac{e\u3008\tau \u3009}{{m}^{*}}$. As such, at low temperatures, the Coulomb scattering is proportional to the carrier density in the tri- and four-layer graphene structures [21–23].

_{3-4 layers}∝

*k*

_{ B }

*T*) [21]. For tri- and four-layer graphene, the resistance can be expressed as:

*R*

_{sr−3–4 layers}=

*C*, and A, B and C are the fitting parameters. In our measurements, we have observed a linear approximation for the temperature-dependent normalized resistance of tri- and four-layer graphene:

These considerations explain qualitatively why the resistance of tri- and four-layer graphene decreases with the increasing temperature. We note that due to the complexity of the FLG band structure, these anomalous electrical properties are believed to originate in the unusual band structures near the Fermi level of graphene [26–29]. More rigorous theoretical explanation of FLG intrinsic semiconductor behaviours would be interesting and requires further experimental investigations.

## Conclusions

In conclusion, FLG interconnects were fabricated via a combination of mechanical exfoliation and photo lithography techniques. The temperature dependence of the electrical resistance of tri- and four-layer graphene was investigated. The observed *I-V* curve shows unique combination of the low threshold of linearity and manifestation of the second ohmic region for the strong DC electric field in the FLG interconnects. With the RCDA method, our experimental results suggest that Coulomb interaction plays an essential role. The non-metallic temperature-dependent resistance is observed in the temperature range of 5 to 340 K. In this case, even though the FLG band structure as semimetal with zero-band gap, tri- and four-layer graphene resistors behave more like semiconductors. By combining the Coulomb and short-range scattering theories, an analytical model was developed, which well explains the experimental results.

## Declarations

### Acknowledgments

We would like to acknowledge support from Nanyang Technological University (NTU) (M58040017) and Ministry of Education, Singapore (MOE2011-T2-2-147 and MOE2011-T3-1-005). Y. P. Liu acknowledges Dr Cheong Siew Ann (NTU) for useful discussions. The authors also thank Sun Li and Li Yuanqing for their assistance in experimental measurements.

## Authors’ Affiliations

## References

- Geim AK, Novoselov KS: The rise of graphene.
*Nat Mater*2007, 6: 183. 10.1038/nmat1849View ArticleGoogle Scholar - Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films.
*Science*2004, 306: 666. 10.1126/science.1102896View ArticleGoogle Scholar - Novoselov KS, Geim AK, Morozov SV, Jiang D, Katsnelson MI, Grigorieva IM, Dubonos SV, Firsov AA: Two-dimensional gas of massless Dirac fermions in graphene.
*Nature*2005, 438: 197. 10.1038/nature04233View ArticleGoogle Scholar - Novosetov KS, Jiang Z, Zhang Y, Morozov SV, Stormer HL, Zeitter U, Maan JC, Boebinger GS, Kim P, Geim AK: Room-temperature quantum hall effect in graphene.
*Science*2007, 315: 1379. 10.1126/science.1137201View ArticleGoogle Scholar - Wallace PR: The band theory of graphite.
*Phys Rev*1947, 71: 622. 10.1103/PhysRev.71.622View ArticleGoogle Scholar - Semenoff GW: Condensed-matter simulation of a three-dimensional anomaly.
*Phys Rev Letts*1984, 53: 2449. 10.1103/PhysRevLett.53.2449View ArticleGoogle Scholar - Barone V, Hod O, Scuseria GE: Electronic structure and stability of semiconducting graphene nanoribbons.
*Nano Letts*2006, 6(12):2748. 10.1021/nl0617033View ArticleGoogle Scholar - Berger C, Song Z, Li X, Wu X, Brown N, Naud C, Mayou D, Li T, Hass J, Marchenkov AN, Conrad EH, First PN, de Heer WA: Electronic confinement and coherence in patterned epitaxial graphene.
*Science*2006, 312: 1191. 10.1126/science.1125925View ArticleGoogle Scholar - Latil S, Henrard L: Charge carriers in few-layer graphene films.
*Phys Rev Letts*2006, 97: 036803.View ArticleGoogle Scholar - Aoki M, Amawashi H: Dependence of band structures on stacking and field in layered graphene.
*Sol Stat Comm*2007, 142: 123. 10.1016/j.ssc.2007.02.013View ArticleGoogle Scholar - Lu CL, Chang CP, Huang YC, Chen RB, Lin ML: Influence of an electric field on the optical properties of few-layer graphene with AB stacking.
*Phys Rev B*2006, 73: 144427.View ArticleGoogle Scholar - Gruneis A, Attaccalite C, Wirtz L, Shiozawa H, Saito R, Pichler T, Rubio A: Tight–binding description of the quasiparticle dispersion of graphite and few–layer graphene.
*Phys Rev B*2008, 78: 205425.View ArticleGoogle Scholar - Zhang Y, Tang TT, Girit C, Hao Z, Martin MC, Zettl A, Crommie MF, Shen YR, Wang F: Direct observation of a widely tunable bandgap in bilayer graphene.
*Nature*2009, 459: 820. 10.1038/nature08105View ArticleGoogle Scholar - Kuzmenko AB, Crassee I, van der Marel D, Blake P, Novoselov KS: Determination of the gate-tunable band gap and tight-binding parameters in bilayer graphene using infrared spectroscopy.
*Phys Rev B*2009, 80: 165406.View ArticleGoogle Scholar - Craciun MF, Russo S, Yamamoto M, Oostinga JB, Morpurgo AF, Thrucha S: Trilayer graphene is a semimetal with a gate-tunable band overlap.
*Nat Nanotechnol*2009, 4: 383. 10.1038/nnano.2009.89View ArticleGoogle Scholar - Malard LM, Pimenta MA, Dresselhaus G, Dresselhaus MS: Raman spectroscopy in graphene.
*Phys Rep*2009, 473: 51. 10.1016/j.physrep.2009.02.003View ArticleGoogle Scholar - Calizo I, Bejenari I, Rahman M, Liu G, Balandin AA: Ultraviolet Raman microscopy of single and multilayer graphene.
*J Appl Phys*2009, 106: 043509. 10.1063/1.3197065View ArticleGoogle Scholar - Balev OG, Vasko FT, Ryzhii V: Carrier heating in intrinsic graphene by a strong dc electric field.
*Phys Rev B*2009, 79: 165432.View ArticleGoogle Scholar - Vasko FT, Ryzhii V: Voltage and temperature dependencies of conductivity in gated graphene.
*Phys Rev B*2007, 76: 233404.View ArticleGoogle Scholar - Chuang C, Puddy RK, Lin HD, Lo ST, Chen TM, Smith CG, Liang CT: Experimental evidence for Efros–Shklovskii variable range hopping in hydrogenated graphene.
*Solid State Communications*2012, 152(10):905. 10.1016/j.ssc.2012.02.002View ArticleGoogle Scholar - Zhu WJ, Perebeinos V, Freitag M, Avouris P: Carrier scattering, mobilities, and electrostatic potential in monolayer, bilayer, and trilayer graphene.
*Phys Rev B*2009, 80: 235402.View ArticleGoogle Scholar - Hwang EH, Das Sarma S: Acoustic phonon scattering limited carrier mobility in two-dimensional extrinsic graphene.
*Phys Rev B*2008, 77: 115449.View ArticleGoogle Scholar - Ando T: Anomaly of optical phonon in monolayer graphene.
*J Phys Soc Jap*2006, 75: 7.Google Scholar - Hwang EH, Adam S, Das Sarma S: Carrier transport in two-dimensional graphene layers.
*Phys Rev Letts*2007, 98: 18.Google Scholar - Hwang EH, Das Sarma S: Screening-induced temperature-dependent transport in two-dimensional graphene.
*Phys Rev B*2009, 79: 165404.View ArticleGoogle Scholar - Liu YP, Goolaup S, Murapaka C, Lew WS, Wong SK: Effect of Magnetic Field on the Electronic Transport in Trilayer Graphene.
*Acs Nano*2010, 4: 7087–7092. 10.1021/nn101296xView ArticleGoogle Scholar - Zheng Y, Ando T: Hall conductivity of a two-dimensional graphite system.
*Phys Rev B*2002, 65: 245420.View ArticleGoogle Scholar - Liu YP, Lew WS, Goolaup S, Liew HF, Wong SK, Zhou TJ: Observation of oscillatory resistance behavior in coupled bernal and rhombohedral stacking graphene.
*Acs Nano*2011, 5: 5490–5498. 10.1021/nn200771eView ArticleGoogle Scholar - Yang CH, Peeters FM, Xu W: Density of States and magneto-optical conductivity of graphene in a perpendicular magnetic field.
*Phys Rev B*2010, 82: 205428.View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.